This is an open access article published under an ACS AuthorChoice License, which permits copying and redistribution of the article or any adaptations for non-commercial purposes.
Surface- and Tip-Enhanced Raman Spectroscopy in Catalysis Thomas Hartman,† Caterina S. Wondergem,† Naresh Kumar,†,‡ Albert van den Berg,§ and Bert M. Weckhuysen*,† †
Faculty of Science, Debye Institute for Nanomaterials Science, Utrecht University, Universiteitsweg 99, 3584 CG Utrecht, The Netherlands ‡ National Physical Laboratory, Hampton Road, Teddington, Middlesex TW11 0LW, U.K. § BIOS Lab on a Chip Group and MESA+ Institute for Nanotechnology, University of Twente, P.O. Box 217, 7500 AE Enschede, The Netherlands ABSTRACT: Surface- and tip-enhanced Raman spectroscopy (SERS and TERS) techniques exhibit highly localized chemical sensitivity, making them ideal for studying chemical reactions, including processes at catalytic surfaces. Catalyst structures, adsorbates, and reaction intermediates can be observed in low quantities at hot spots where electromagnetic ﬁelds are the strongest, providing ample opportunities to elucidate reaction mechanisms. Moreover, under ideal measurement conditions, it can even be used to trigger chemical reactions. However, factors such as substrate instability and insuﬃcient signal enhancement still limit the applicability of SERS and TERS in the ﬁeld of catalysis. By the use of sophisticated colloidal synthesis methods and advanced techniques, such as shell-isolated nanoparticle-enhanced Raman spectroscopy, these challenges could be overcome.
atalysis is essential in the ﬁeld of sustainable chemistry because it allows reactions to take place more quickly, eﬃciently, and safely.1−3 To improve chemical processes it is crucial to know how catalysts operate and how, why, and when they cease to work. Understanding the mechanism of all involved surface reactions in the case of heterogeneous catalysts is the key to designing the best possible catalytic materials. For this purpose, researchers use a wide variety of techniques. They originally used methods to study catalysts before and after reaction, such as spectroscopy, (electron) microscopy, and many more. Although these methods have greatly enhanced the understanding of catalysts, knowledge of actual operating catalysts remains incomplete. Understanding working catalysts requires the use of techniques that are able to identify when and where reactions take place, ultimately linking this information to the catalytic performance of these materials. Valuable techniques for elucidating molecular structures are vibrational spectroscopy methods, including various forms of infrared (IR)4−6 and Raman spectroscopy.7−10 Raman spectroscopy enables the measurement of vibrational energy levels, which provide information about the molecular composition and structure within a sample. Operative under several diﬀerent conditions, this spectroscopic technique has greatly improved the knowledge of both the syntheses7,8 and operation9,10 of catalytic solids. However, Raman spectroscopy lacks sensitivity due to the small Raman scattering cross section of analyte molecules.11 The sensitivity of Raman spectroscopy can be enhanced using specialized techniques, of which resonance Raman,11−14 coherent anti-Stokes Raman
© 2016 American Chemical Society
spectroscopy (CARS),15 and surface-enhanced Raman spectroscopy (SERS) are the three most popular choices.16 All of these techniques have their own strengths and weaknesses, but compared to the others, SERS exhibits a strong feature for catalysis: highly localized sensitivity. This local sensitivity can be exploited to sense surface species and adsorbates.17−19 Multiple techniques, such as CARS and SERS, can be combined to obtain even stronger signal intensities.20 However, SERS is not the only surface-sensitive vibrational spectroscopic technique used in the ﬁeld of catalysis. For example, other characterization techniques to study surface adsorbates include polarization modulation infrared reﬂection absorption spectroscopy (PM-IRRAS)21,22 and sum frequency generation (SFG).23−25 The latter approach has been pioneered by the group of Somorjai, and has been used, for example, to investigate the hydrogenation of benzene over platinum single crystals with a combined high-pressure scanning tunneling microscopy (HP-STM) and SFG instrument.26 On the other hand, SERS enables the observation and characterization of the structure of surface species and adsorbates with greater sensitivity up to the level of detecting single molecules. When combined with scanning probe microscopy (SPM) methods, tip-enhanced Raman spectroscopy (TERS) can even reach nanoscale spatial resolution.27 Furthermore, the SERS substrates can be triggered to start a reaction due to the formation of the strong electric ﬁeld, hot Received: January 22, 2016 Accepted: March 31, 2016 Published: April 14, 2016 1570
DOI: 10.1021/acs.jpclett.6b00147 J. Phys. Chem. Lett. 2016, 7, 1570−1584
The Journal of Physical Chemistry Letters
Figure 1. Strongest EFs arise from hot spots, which are produced by gap-mode plasmons that emerge between closely spaced plasmonic particles or tip−surface interactions where the plasmons overlap. (a) The Raman signal EF can reach theoretical values of 108 for dimer gold nanoparticles under 559 nm laser irradiance40 and (b) 1011 for a sharp gold tip−gold surface interaction under 633 nm laser irradiance.40 (c) The electric ﬁeld is at its strongest when the particles touch and rapidly reduces to a negligible value when the particles are more than 15 nm away from each other. (d) This can be observed in the SERS spectra of adsorbed ammonium salt of pyrene on Ag@SiO2 spheres. (e) Plot of SERS EF versus distance between the particles.41 Reprinted with permission from ref 40. Copyright 2008 Royal Society of Chemistry. Reprinted from ref 41. Copyright 2012 American Chemical Society.
electrons, and the involved heat generation.28,29 With increased control over these SERS substrates, improved Raman signals are obtained with shorter acquisition times, allowing the observation of possible reaction intermediates or even transition states.30,31 A few hurdles need to be overcome before SERS and TERS can become a routine analytical tool for catalysis. In this Perspective, we brieﬂy introduce the capabilities and challenges of SERS and TERS and present several examples of past work and future perspectives to encourage readers to start working with and expand the knowledge of these powerful analytical tools for the study of catalytic reactions. Although this Perspective is mostly aimed at heterogeneous catalysis, it is important to realize that the strengths of SERS are not necessarily limited to this ﬁeld of research and can also be applied to the ﬁeld of homogeneous catalysis.32,33 Furthermore, SERS is promising to become one of the tools of choice for monitoring the dynamics of biological macromolecules in biomedical applications and is useful for the characterization of biocatalysts, although its current main use is in diagnostics.34,35 SERS. The strong Raman signal enhancement in SERS arises from the excitation of a localized surface plasmon in metallic nanostructures by an external oscillating electric ﬁeld that matches the resonant frequency of the plasmon. Metallic nanoparticles are polarized by the electric ﬁeld, and the induced dipole will resonate with the frequency of the incident light. This phenomenon is known as a “localized surface plasmon resonance” (LSPR) and creates a strong localized electromagnetic ﬁeld, which strongly enhances the Raman signal from analyte molecules in close vicinity of the metallic nanoparticles. The strength of SERS signals dissipates by r−10 to r−12, depending on the substrate and analyte.17−19,36,37 This distance dependency makes the technique an ideal surface-speciﬁc characterization technique. SERS substrates are often fabricated from gold and silver nanoparticles. Depending on their size, shape, aggregation state, and the properties of the excitation laser, the Raman signal can be enhanced by over a factor of 106.17−19,31,38 Silver
nanoparticles provide stronger SERS signals than gold nanoparticles; however, gold nanoparticles are often preferred because of their higher stability.39 Indeed, gold nanoparticles are more stable than their silver counterparts and are therefore easier to handle and store. Additionally, they are more likely to retain their SERS activity during experiments requiring elevated temperatures and/or pressures. However, because silver nanoparticles are more SERS active for laser excitation below 600 nm, they provide stronger signal enhancement since Raman scattering intensity is proportional to λ−4. The strongest signal enhancements in SERS substrates are obtained from so-called “hot spots”, sites that have the strongest LSPR. For example, at the junction between a nanoparticle with another nanoparticle or a bulk metal surface, the surface plasmons can overlap to form gap-mode plasmons (Figure 1a,b). Depending on the distance between the particles, these gap-mode plasmons tremendously enhance the signal intensity in comparison to single particles, and it vanishes quickly when they move away from each other (Figure 1c−e).40,41 This knowledge of hot spots illustrates the diﬃculty of applying SERS to other catalysts besides silver, gold, and copper. Since the highest enhancements come from between two plasmonic particles, one of the largest challenges becomes the observation of surface species and adsorbates on other catalytic materials. Micro- and Nanostructured SERS Surfaces. Nanoparticlebased SERS oﬀers advantages in terms of ease of preparation and control of chemistry, but has limited reproducibility due to surface inhomogeneity, varying dimer orientation, and illdeﬁned dimer spacing. For over a decade eﬀorts have been made to create SERS surfaces with well-deﬁned and homogeneously distributed hot spots using a variety of methods such as nanoimprinting, e-beam lithography, focused ion beam (FIB) milling, laser interference lithography (LIL), and template-based technologies that are much more promising.42,43 Of these methods, photolithography holds great promise because of its exact geometric control and availability of an extensive technological toolbox. With this 1571
DOI: 10.1021/acs.jpclett.6b00147 J. Phys. Chem. Lett. 2016, 7, 1570−1584
The Journal of Physical Chemistry Letters
Figure 2. (a) Nano v-grooves,46 (b) artist’s impression of nanopyramids,46 (c) nanowires and nanogaps with cross section in inset,45 (d) histogram of analytical enhancement factor (AEF) on a nanowire−nanogap substrate,45 (e) −0.2 V and (f) −0.5 V spectro-electrogram of MPY/ hemin modiﬁed gold nanowire electrodes with the Fe2+ and Fe3+ bands indicated.48 Reprinted from refs 45, 46, and 48. Copyright 2013, 2010, and 2015, respectively, American Chemical Society.
bands upon using a Ag/AgCl reference electrode and a platinum counter electrode. It was found that when the redox state of the hemin group of the mercaptopyridine (MPy)/ hemin modiﬁed gold nanowires was changed by shuttling the voltage between −0.2 V (Figure 2e) and −0.5 V (Figure 2f) versus Ag/AgCl, a corresponding change in the SERS spectra was observed.48 This demonstrates that a combination of orthogonal analytical techniques combined with dynamic control of environmental conditions using microﬂuidics clearly holds great promise for in situ study of catalytic reactions. Combining SERS and Catalysis. Gold and silver metal nanoparticles show catalytic behavior in a variety of reactions, implying that they can simultaneously act as sensor as well as catalyst.49,50 Gold and silver catalysts can generally be used in three diﬀerent types of surface reactions: heterogeneous catalysis,51 electrochemical reactions,47 and photocatalytic (plasmon-driven) reactions.52−54 Valuable industrial reactions, such as NOx reduction,55 epoxidation reactions,50,56 and methanol synthesis57 can be carried out over copper and silver metals. However, because of their lower stability in air, they are less implemented in SERS in comparison to gold nanoparticles. Alloys made from silver/gold or copper/gold often have higher stability than pure materials. Gold−silver alloys can be fabricated for example by a simple coreduction of HAuCl4 and AgNO3 using trisodium citrate.58 Star-shaped copper/gold alloys have been prepared as well by a coreduction using glucose as reductant.59 The introduction of other metals during the synthesis to prepare alloyed nanoparticles not only is interesting to increase the stability, but also will aﬀect the position of the LSPR as well as catalytic activity.60 A recent study by Marimuthu et al. showed that the oxidation state of surface atoms in copper nanoparticles can
technique, structures such as nanogroove, nanopyramid, and nanogap−nanowire arrays have been recently realized with tunable gap spacing and high spatially averaged analytical enhancement factors (AEF),44 as shown in Figure 2.45,46 Since in the ﬁrst two of these approaches LIL is used in combination with anisotropic (100) silicon etching to create nanometer pitches and spacing, no mask is needed and the method is therefore relatively cheap. However, a disadvantage of these anisotropically etched structures is that the SERS hot spots with high signal enhancement occur only at a very small percentage of the surface area because the groove width and spacing between the pyramid sidewalls vary strongly. The third structure, the nanogap−nanowire, is particularly interesting for two reasons. First, the gap size remains constant (